Black painted pottery, Kildehuse II, Odense County, Denmark.
This work aimed at characterization of a black layer covering a Bronze Age (period VI) pot surface. To solve research problems plane polarized light microscopy (PLM), scanning microscopy with X-ray microanalyser (SEM/EDS), Raman and FTIR microspectroscopies were applied. Observation of the black layer under the PLM suggests that we deal with an opaque, isotropic layer, purposely put on leather-hard, burnished surface of a pot. No traces of organic substances that might have modified a pot surface before painting were detected. The black layer coats the pot with a continuous 0.2-0.4 μm thick layer. The black layer must have been applied while warm or hot. It is recognized that the black layer is a true painting layer. Spectroscopic analyses (Raman and FTIR) point that birch tar or a birch-pine tar had been applied. Carbon black should be definitely excluded. The analyzed organic substance is structurally ordered in various degrees, due to varying temperature influence. Some Raman spectra reveal, in second-order region of the spectrum (>2000 cm(-1)), the graphite presence. Scarce points reveal the presence of inorganic admixtures: clay minerals, feldspars and quartz. The next question is: Is it an organic paint or a carbon-based, "mixed" paint? Inorganic admixtures are only casual. Relatively high concentration of alumina is expected to have appeared due to aluminum mobility in acidic environment and this was provided by organic tar/pitch substances. Phosphorus (usually with calcium) mostly concentrates together with clay minerals. Thus, hypothesis on bone powder or ash addition to tar/pitch should be excluded. Some elements may originate not only from inorganic substances but also from wood ashes.
Rzeszów University, Institute of Archaeology, Hoffmanowej 8 Str, Rzeszów, Poland. joanna.trabska@archeologia.rzeszow.pl
Joanna
J
Trąbska
Aleksandra
A
Wesełucha-Birczyńska
Janina
J
Zięba-Palus
Mads Thagård
MT
Runge
D000538:Aluminum Silicates / Q000032:analysis*; D029662:Betula / Q000737:chemistry; D000077215:Clay; D003718:Denmark; D005843:Geography; D008859:Microscopy, Polarization; D010150:Paint / Q000032:analysis*; D013052:Spectrometry, X-Ray Emission; D017550:Spectroscopy, Fourier Transform Infrared; D013059:Spectrum Analysis, Raman; D013499:Surface Properties
D000538:Aluminum Silicates; D000077215:Clay